EXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS


 Alan Nicholson
 1 years ago
 Views:
Transcription
1 EXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS Kevin L. Peil +, Ever J. Barbero +, Eduardo M. Sosa* + Department of Mechanical and Aerospace Engineering, West Virginia University (WVU), Morgantown, West Virginia, USA *Department of Civil and Environmental Engineering, West Virginia University (WVU), Morgantown, West Virginia, USA The development of Finite Element Models (FEM) of inflatable structures made from woven webbings used to seal conduits and large pipes with irregular shapes requires not only the typical material properties such as modulus of elasticity, axial strength, density, and Poisson's ratio, but also an estimation of the shear behavior to account for the drapeability of the inflatable necessary to conform to the irregularities of the section to be sealed. Because the fibers in woven webbings are not continuous along the two principle directions, a priori it is not possible to calculate analytically the shear properties based on the fiber elastic modulus and Poisson s ratio. Due to this limitation, mechanical testing is necessary to determine the shear behavior. An experimental methodology for determining the shear characteristics of woven webbings is proposed. Experimental methods are developed for testing the materials using the denominated "picture frame" designed to produce a shearing effect from an axial force. These frames allow the materials to be stressed biaxially prior to the shear testing to observe the shear performance under similar axial stress states, which will be seen in the material for specific applications. Testing yields load and displacement data, which can be used to determine the shear modulus as a function of the materials angular displacement. The Department of Homeland Security, Science and Technology Directorate, Infrastructure Protection and Disaster Management Division provided funding support for this research. 1. INTRODUCTION The shear characteristics of fabrics have been analyzed in a number of ways ranging from mathematical models, which predict the material behavior based on fiber geometry and friction coefficients, to mechanical testing, which directly measures a materials bulk resistance to shear deformation [1][2]. The shear mechanisms influence the draping and pliability of a fabric and determine the ability of the material to conform to a three dimensional surface [1]. The ability of a fabric to conform to a doublecurvature surface depends mainly on the inplane shear behavior [3]. Because the fibers within a webbing are not continuous and are not connected along any two principle directions, the materials cannot be considered isotropic or homogeneous. These types of micromaterials can also display nonlinear and unpredictable behavior under multiple stress states. Because of this, a theoretical analysis can become very complex or impossible and experimental determination of the material behavior becomes necessary. The shear properties of webbings will be dependent on the biaxial state of stress, which the material will be under. The material must be tested in a manner where the tensile and shear forces can be applied simultaneously [4].
2 Material Selection Two materials, nylon and Vectran, HT, were used to categorize the shear behavior of the woven outer layer of the inflatable structure being analyzed in the FEM. The use of two materials was necessary due to the limited supply of Vectran available for testing. The nylon webbings that were used had the same width and thickness as Vectran and similar coefficients of friction. The principle difference between the two materials is the ultimate tensile strength. A table summarizing the key properties of the two materials is shown in Table 1. Because the mechanisms of shear are a function of weave pattern, friction coefficient, and pretensioning, and are roughly independent of the tensile strength of the individual fibers [1], conclusions on the shear characteristics of the outer layer of the inflatable structure could be drawn from tests run using both materials. Table 1: Material properties of Nylon and Vectran HT webbings Width Thickness Coefficient of Ultimate Tensile friction Strength Weave pattern Nylon 2 inches 0.1 inch ~0.5 7,000 lb herringbone Vectran 2 inches 0.1 inch ~0.5 24,000 lb herringbone Material Preparation Twelve strips were initially cut from a bulk roll of material to be woven together to form a representative volume element (RVE) of a section of the inflatable structure being analyzed. The weave pattern used was a square weave. Strips were cut 27 inches in length to allow for attachment to the picture frame shear test stand and pretensioning pulley system. A smaller RVE could have been used to measure the shear behavior of the material under small angular displacements (020 degrees), however jamming of the fibers and wrinkling of the material, which occurred at large angular displacements (2036 degrees), would not have been observable. Samples were prepared under dry conditions at ambient air temperatures. Picture Frame Shear Test Stand Preparation Figure 2: CAD image of picture frame shear test stand A picture frame shear test stand was used to apply the shearing loads to the sample during testing. A computeraided design (CAD) image of the frame that was built is shown in figure 2. The arms of the frame measured nineteen inches in length, two inches wide and one inch thick. The design of the frame allowed the material to be pretensioned along each principle direction prior to attachment, permitting the measurement of shear under a biaxial state of stress. While in the frame, the strips of material were held in place using a dead man system, which uses the materials self friction to hold the bottom of each strip in the frame and a steel plate secured with bolts to hold the top of each strip. Because of the design of the frame, while the material was being sheared, the
3 distance between any two colinear connection points would remain equidistant. This allowed the biaxial stress state in the material to remain constant during testing. The frame was constructed using halfinch thick 304 stainless steel plate. The pivot bearings were made from smoothed, oneinch diameter, solid stainlesssteel shafts cut four inches long. Between the steel arm plates were thin Vectran shims used to ensure uniform contact along the length of the frame. 2. EXPERIMENTATION Material PreTensioning Pretensioning of the webbing strips began with attachment of the bottom of each strip to the shear test frame using a dead man gripping method. Six strips of webbing material were laid side by side on top of the disassembled shear test frame, perpendicular to the length of the bottom arm with two inches of overhang. The overhang of each strip was then folded over top of a halfinch, plain carbon steel rod and held in place using four staples. Once all six webbings were folded over the rod, Vectran shims were laid across the length of the arm to assure even contact with the steel holding plate. The top of the shear test frame arm was then attached over the folded webbings. The top of each webbing strip was then attached to a specially designed pretensioning pulley system. The pulley system was comprised of three twoinch diameter wheels spaced four inches apart from one another. The wheels were mounted on a set of steel plates, which allowed independent movement of each wheel relative to one another. Steel cables with attached mounting plates were then wrapped over the pulleys for attachment to the top end of each webbing strip. Due to the design of the pulley system and the method of attachment, when a tensile load was applied to the top arm of the system the load would be equally distributed to each webbing, resulting in a uniform stress across the width of the sample. Figure 3: Vectran sample attached to pulley system and frame for pretensioning Figure 3: Vectran sample attached to pulley system and frame for pretensioning To apply the required pretensioning load, the pulley system and shear test frame were connected to an Instron HDX1000 tensile test machine. Connections were made to the machine via two oneinch diameter steel shafts, which were attached to solid steel blocks held in place using the machines hydraulic wedge grips. The pulley system was initially lifted into place and secured to the top bolt. The bottom crosshead on the tensile test machine was then raised into position to attach to the bottom of the shear test frame. An image of the pulley system and shear test frame attached to the tensile test machine with Vectran webbings at the pretensioning stage can be seen in figure 3.After attachment to the tensile test machine, the system was tensioned to approximately 600 pounds per webbing and held at this load for 10 minutes to allow for stress relaxation within the system. A top holding plate was secured to the ends of the webbings using 12 bolts. Attachment of the holding plate required all components to be held tightly in place using four Cclamps and wedges.
4 Had the material not been held tightly in place, as the fibers were broken by the drill to produce bolt holes, they would have been pulled down within the frame resulting in a local loss of tension in the vicinity of each bolt. This would have resulted in prematuree wrinkling of the sample as well as an overall inaccuracy in the representation of the material layer that was to be modeled. Once attachment had been completed, the shear test frame and pulley system were removed from the tensile test machine and the excess material connecting the shear test frame to the pulley system was cut. The procedure was repeated for the set of perpendicular webbings resulting in a representative volume element of the woven outer layer of the inflatable structure being held in place within the shear test frame under a uniform biaxial state of stress. Shear Testing of the Prepared Sample After sample preparation and detachment from the pulley system, the shear test frame was reattached to the tensile test machine from two pivot points on opposite corners of the frame. Using Instron s Partner software, a program was written that would move the top bearing of the shear frame upward at a rate of 0.02 inches per second. The program recorded crosshead displacement, load on the frame, and time. The displacement of the top of the frame resulted in the material being deformed into a diamond shape, shearing the material as the frame was displaced. From the data collected, the nominal shear stress in the material and the angular displacement of the fibers could be calculated. Each sample was sheared five times to an angular displacement of approximately 36 degrees. Tests were stopped when large amounts of wrinkling were observed. An image of a sheared sample of nylon is shown in figure 4. Figure 4: Images of Nylon sample under varying angles of shear deformation 3. RESULTS Analysis of shear was done in a manner that would yield results usable within the FEM of the inflatable structure being investigated. The model was developed using Abaqus software, which requires an input plot of nominal shear stress versus fiber change in angle [5]. As such, this information was calculated and plotted based on the deformation of the frame and the required load to cause the deformation. After plotting the results from each test, the values were averaged to form a single representative plot of nominal shear stress versus fiber change in angle.
5 Each test had a slight difference in the amount of measured preload after sample attachment. This was due to fiber slippage caused by the holes that were drilled for attachment and tightening of the interface between the top steel holding plates and the top arm of the shear test frame. The recorded initial preloads and loads after attachment for each of the principle directions are supplied in table 2. The experimental setup of the tests was seen to be a major factor in the accuracy of each trial. Sample placement within the frame must be exact to assure the material is sheared properly. All connections along the frame for securing the webbing materials must be made while minimizing any fiber slippage to maintain a uniform preload along the length of the sample. Material was monitored during testing to assure damage was not induced as a result of over deformation. Table 2: Material Preload in the two principle directions Sample Initial Preload (direction 1) Load after attachment (direction 1) Load per webbing Initial Preload (direction 2) Load after attachment (direction 2) Load per webbing Sample 1 (Nylon) Sample 2 (Nylon) Sample 3 (Nylon) Sample 4 (Nylon) Sample 5 (Vectran) 4000 lb 2860 lb 477 lb 4000 lb 2780 lb 463 lb 4000 lb 3180 lb 530 lb 4000 lb 3264 lb 544 lb 4000 lb 3280 lb 547 lb 4000 lb 3411 lb 569 lb 4000 lb 3500 lb 583 lb 4000 lb 3500 lb 583 lb 4900 lb 4174 lb 696 lb 4900 lb 4500 lb 750 lb The frame geometry, deflection, and data from each test were used to calculate webbing change in angle. Knowing that the initial distance between two opposite pivot points on the frame was inches in the undeformed (i.e., square) configuration and that the side length of each arm between each pivot point was 19 inches, equation 1 could be used to determine the change in angle of the webbings as a function of the crosshead displacement at any given time. Figure 5 shows a schematic of the information needed from the tests frame to perform the calculations.
6 L F w w θ Figure 5: Schematic of picture frame shear test pertinent information The nominal shear stress (T 12 ) in the material is calculated as a function of material thickness, width of the sample, applied load, and angular displacement. Nominal shear stress was calculated using equation 2. Equation 1: θ = 90 2 cos. F Equation 2: T = Where L is the displacement of the tensile test machine crosshead, F is the applied load to the frame as measured by the tensile test machine, t is the material thickness of.2 inch, w is the edge width of the sample (12 inches) and θ is the angular displacement of the webbings. Data produced by the tensile test machine were reduced using MATLAB, producing figure 6 showing the results from each trial.
7 Figure 6: Complete results of each trial. A more compact and easily understood plot was produced by taking the average of all trials for each test. Best fit curves were mathematically forced through the origin in accordance with experimental observations. A plot of the averages from each test can be seen in Figure 7. Figure 7: Averaged results for each test From the above results, points can be chosen to represent key elements of the curve that define the shear behavior. For the FEA model, 12 points were used, each separated by three degrees. There are four shearing mechanisms that can be observed from the results. Under angular displacements between zero and 2.5 degrees, the deformation of the material is too small to overcome the friction between the strips of webbing. As such, the material acts as a rigid body
8 and the slope representing the shear modulus is large. Between 2.5 and 20 degrees of angular displacement, there is yarn slippage at the intersection and elastic bending resulting in the flattening of the curve. At angles above 20 degrees, there is jamming and wrinkling within the material requiring larger shear stresses to produce the displacements. The final plot used to define the material shear behavior can be seen in figure 8. Figure 8: Data points defining the material shear behavior for Vectran and Nylon The tests showed a large amount of variability between samples, speculatively due to the differences in preload between tests. Fiber micromechanic behavior was an additional source of variability, due to the differences in tension across the width of the sample caused by fiber slippage during sample attachment. Future work will be done to visually map the individual changes in webbing angle using digital image correlation, which will then be compared with equation 1 to determine the accuracy of the assumption that the webbing change in angle is equal to that of the frame. As shear deformation angle increases and jamming of the material occurs, angular displacements of the webbings in the vicinity of the intersection points were seen to be larger than that of the bulk of the surface. These intersections will require further study and evaluation to determine the stress state at these points. 4. CONCLUSIONS The use of a picture frame shear test stand was seen as a viable method for evaluating the shear characteristics of a woven material. The ability to pretension a fabric sample prior to shear testing is required due to the nature of the fiber interactions as the sample is displaced. Experimental measurement of the shear performance of fabrics is required as no method for accurately calculating the behavior is available. Tests must be performed under the same state of
9 biaxial stress, which will be seen by the material when in use. Friction between fibers was seen to be the primary mechanism for shear resistance. Evaluation of the results indicates that the outer layer of the inflatable structure will show little resistance to shear deformation as is required for the structure to conform to irregularities within the conduits it will be housed within. 5. REFERENCES 1. Grosberg, P., Park, B.J., The mechanical properties of woven fabrics. Part V. The initial modulus and the frictional restraint in shearing of plain weave fabrics. Textile Res J 1966;36: Domskiene, J., Strazdien, E., Investigation of fabric shear behavior. Fibres &Textiles in Eastern Europe April/June 2005, Vol.13 No.2(50) 3. Potluri, P., Ciurezu, D. Young, R. Biaxial shear testing of textile performs for formability analysis. 16 th International Conference on Composite Materials Basset, R., Postle, R., Experimental methods for measuring fabric mechanical properties: A review and analysis. Textile Res J. 69(11), (1999) 5. L. Dong, C. Lekakou and M. G. Bader, Processing of Composites: Simulations of the Draping of Fabrics with Updated Material Behaviour Law. Journal of Composite Materials : Abaqus 6.8. User Manual 7. Sun, H., Pan, N., Shear deformation analysis for woven fabrics. Composite Structures 67(2005)
Tuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationEquilibrium & Elasticity
PHYS 101 Previous Exam Problems CHAPTER 12 Equilibrium & Elasticity Static equilibrium Elasticity 1. A uniform steel bar of length 3.0 m and weight 20 N rests on two supports (A and B) at its ends. A block
More informationExperiment Two (2) Torsional testing of Circular Shafts
Experiment Two (2) Torsional testing of Circular Shafts Introduction: Torsion occurs when any shaft is subjected to a torque. This is true whether the shaft is rotating (such as drive shafts on engines,
More informationChapter 12. Static Equilibrium and Elasticity
Chapter 12 Static Equilibrium and Elasticity Static Equilibrium Equilibrium implies that the object moves with both constant velocity and constant angular velocity relative to an observer in an inertial
More informationInitial Stress Calculations
Initial Stress Calculations The following are the initial hand stress calculations conducted during the early stages of the design process. Therefore, some of the material properties as well as dimensions
More informationCONNECTION DESIGN. Connections must be designed at the strength limit state
CONNECTION DESIGN Connections must be designed at the strength limit state Average of the factored force effect at the connection and the force effect in the member at the same point At least 75% of the
More informationStrength of Material. Shear Strain. Dr. Attaullah Shah
Strength of Material Shear Strain Dr. Attaullah Shah Shear Strain TRIAXIAL DEFORMATION Poisson's Ratio Relationship Between E, G, and ν BIAXIAL DEFORMATION Bulk Modulus of Elasticity or Modulus of Volume
More informationSize Effects In the Crushing of Honeycomb Structures
45th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics & Materials Conference 1922 April 2004, Palm Springs, California AIAA 20041640 Size Effects In the Crushing of Honeycomb Structures Erik C.
More informationMicromeso draping modelling of noncrimp fabrics
Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are
More informationTask 1  Material Testing of Bionax Pipe and Joints
Task 1  Material Testing of Bionax Pipe and Joints Submitted to: Jeff Phillips Western Regional Engineer IPEX Management, Inc. 20460 Duncan Way Langley, BC, Canada V3A 7A3 Ph: 6045348631 Fax: 6045347616
More informationDECLARATION. Supervised by: Prof Stephen Mutuli
DECLARATION The work presented in this project is the original work, which to the best of our knowledge has never been produced and presented elsewhere for academic purposes... EYSIMGOBANAY K. J F18/1857/006
More information1. A pure shear deformation is shown. The volume is unchanged. What is the strain tensor.
Elasticity Homework Problems 2014 Section 1. The Strain Tensor. 1. A pure shear deformation is shown. The volume is unchanged. What is the strain tensor. 2. Given a steel bar compressed with a deformation
More informationSTATICS. Friction VECTOR MECHANICS FOR ENGINEERS: Eighth Edition CHAPTER. Ferdinand P. Beer E. Russell Johnston, Jr.
Eighth E 8 Friction CHAPTER VECTOR MECHANICS FOR ENGINEERS: STATICS Ferdinand P. Beer E. Russell Johnston, Jr. Lecture Notes: J. Walt Oler Texas Tech University Contents Introduction Laws of Dry Friction.
More informationSTRESS. Bar. ! Stress. ! Average Normal Stress in an Axially Loaded. ! Average Shear Stress. ! Allowable Stress. ! Design of Simple Connections
STRESS! Stress Evisdom! verage Normal Stress in an xially Loaded ar! verage Shear Stress! llowable Stress! Design of Simple onnections 1 Equilibrium of a Deformable ody ody Force w F R x w(s). D s y Support
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 1
MECE 3321 MECHANICS O SOLIDS CHAPTER 1 Samantha Ramirez, MSE WHAT IS MECHANICS O MATERIALS? Rigid Bodies Statics Dynamics Mechanics Deformable Bodies Solids/Mech. Of Materials luids 1 WHAT IS MECHANICS
More informationExperimental Investigation of SoilPipe Friction Coefficients for Thermoplastic Pipes Installed in Selected Geological Materials
North American Society for Trenchless Technology (NASTT) NASTT s 2014 NoDig Show Orlando, Florida April 1317, 2014 MMT603 Experimental Investigation of SoilPipe Friction Coefficients for Thermoplastic
More informationElastic Properties of Solids Exercises I II for one weight Exercises III and IV give the second weight
Elastic properties of solids Page 1 of 8 Elastic Properties of Solids Exercises I II for one weight Exercises III and IV give the second weight This is a rare experiment where you will get points for breaking
More informationAPI 11E  Specification for Pumping Units
API 11E  Specification for Pumping Units 5 Beam Pump Structure Requirements 5.1 General Requirements for beam pump structures are specified in the following sections. Only loads imposed on the structure
More informationMEMS Project 2 Assignment. Design of a Shaft to Transmit Torque Between Two Pulleys
MEMS 029 Project 2 Assignment Design of a Shaft to Transmit Torque Between Two Pulleys Date: February 5, 206 Instructor: Dr. Stephen Ludwick Product Definition Shafts are incredibly important in order
More informationMECHANICS OF MATERIALS. Prepared by Engr. John Paul Timola
MECHANICS OF MATERIALS Prepared by Engr. John Paul Timola Mechanics of materials branch of mechanics that studies the internal effects of stress and strain in a solid body. stress is associated with the
More informationA FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE
A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
More informationDetermine the resultant internal loadings acting on the cross section at C of the beam shown in Fig. 1 4a.
E X M P L E 1.1 Determine the resultant internal loadings acting on the cross section at of the beam shown in Fig. 1 a. 70 N/m m 6 m Fig. 1 Support Reactions. This problem can be solved in the most direct
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationRock Slope Analysis Small and Large Scale Failures Mode of Failure Marklands Test To establish the possibility of wedge failure. Plane failure is a special case of wedge failure. Sliding along
More informationPLAT DAN CANGKANG (TKS 4219)
PLAT DAN CANGKANG (TKS 4219) SESI I: PLATES Dr.Eng. Achfas Zacoeb Dept. of Civil Engineering Brawijaya University INTRODUCTION Plates are straight, plane, twodimensional structural components of which
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationNUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION
NUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION Fabrice PIERRON*, François CERISIER*, and Michel GRÉDIAC** * SMS/ Département Mécanique et Matériaux, École Nationale Supérieure
More information4.MECHANICAL PROPERTIES OF MATERIALS
4.MECHANICAL PROPERTIES OF MATERIALS The diagram representing the relation between stress and strain in a given material is an important characteristic of the material. To obtain the stressstrain diagram
More informationINFLUENCE KINDS OF MATERIALS ON THE POISSON S RATIO OF WOVEN FABRICS
ISSN 18466168 (Print), ISSN 18485588 (Online) ID: TG217816142553 Original scientific paper INFLUENCE KINDS OF MATERIALS ON THE POISSON S RATIO OF WOVEN FABRICS Željko PENAVA, Diana ŠIMIĆ PENAVA, Željko
More informationMechanics of Solids. Mechanics Of Solids. Suraj kr. Ray Department of Civil Engineering
Mechanics Of Solids Suraj kr. Ray (surajjj2445@gmail.com) Department of Civil Engineering 1 Mechanics of Solids is a branch of applied mechanics that deals with the behaviour of solid bodies subjected
More informationFIS Specifications for Flex Poles (Edition May 2008) Original Text: German
FIS Specifications for Flex Poles (Edition May 2008) Original Text: German 1 Field of Application and Basic Information The following FIS specifications for flex poles are intended to ensure that flex
More informationStatic and Time Dependent Failure of Fibre Reinforced Elastomeric Components. Salim Mirza Element Materials Technology Hitchin, UK
Static and Time Dependent Failure of Fibre Reinforced Elastomeric Components Salim Mirza Element Materials Technology Hitchin, UK Introduction Fibre reinforced elastomers are used in many applications,
More informationPhysical Properties Testing Technical Bulletin
Technical Bulletin MANUFACTURER Raven Lining Systems 13105 E. 61 st Street, Suite A Broken Arrow, OK 74012 (918) 6150020 TENSILE TESTING OF PLASTICS ASTM D638, ISO 527 Tensile tests measure the force
More informationRigid pavement design
Rigid pavement design Lecture Notes in Transportation Systems Engineering Prof. Tom V. Mathew Contents 1 Overview 1 1.1 Modulus of subgrade reaction.......................... 2 1.2 Relative stiffness
More informationENCOMPASSING ROTARYDRAWTUBE BENDING PROCESS WITH SHEET METAL ROLLING BY THREEROLLPUSHBENDING
Int. J. Mech. Eng. & Rob. Res. 015 Harshdeep Singh Sandhu, 015 Research Paper ISSN 78 0149 www.ijmerr.com Vol. 4, No., April 015 015 IJMERR. All Rights Reserved ENCOMPASSING ROTARYDRAWTUBE BENDING PROCESS
More informationSupplementary Information to the article entitled: Internally Architectured Materials with Directionally Asymmetric Friction
Supplementary Information to the article entitled: Internally Architectured Materials with Directionally Asymmetric Friction Ehsan Bafekrpour 1,2, Arcady Dyskin 3, Elena Pasternak 4, Andrey Molotnikov
More informationUNIVERSITY PHYSICS I. Professor Meade Brooks, Collin College. Chapter 12: STATIC EQUILIBRIUM AND ELASTICITY
UNIVERSITY PHYSICS I Professor Meade Brooks, Collin College Chapter 12: STATIC EQUILIBRIUM AND ELASTICITY Two stilt walkers in standing position. All forces acting on each stilt walker balance out; neither
More informationDeflections and Strains in Cracked Shafts due to Rotating Loads: A Numerical and Experimental Analysis
Rotating Machinery, 10(4): 283 291, 2004 Copyright c Taylor & Francis Inc. ISSN: 1023621X print / 15423034 online DOI: 10.1080/10236210490447728 Deflections and Strains in Cracked Shafts due to Rotating
More informationThe Relationship between the Applied Torque and Stresses in PostTension Structures
ECNDT 6  Poster 218 The Relationship between the Applied Torque and Stresses in PostTension Structures Fui Kiew LIEW, Sinin HAMDAN * and Mohd. Shahril OSMAN, Faculty of Engineering, Universiti Malaysia
More informationBE Semester I ( ) Question Bank (MECHANICS OF SOLIDS)
BE Semester I ( ) Question Bank (MECHANICS OF SOLIDS) All questions carry equal marks(10 marks) Q.1 (a) Write the SI units of following quantities and also mention whether it is scalar or vector: (i)
More informationSymmetric Bending of Beams
Symmetric Bending of Beams beam is any long structural member on which loads act perpendicular to the longitudinal axis. Learning objectives Understand the theory, its limitations and its applications
More informationD e s i g n o f R i v e t e d J o i n t s, C o t t e r & K n u c k l e J o i n t s
D e s i g n o f R i v e t e d J o i n t s, C o t t e r & K n u c k l e J o i n t s 1. Design of various types of riveted joints under different static loading conditions, eccentrically loaded riveted joints.
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationDEFLECTION OF BEAMS WlTH SPECIAL REFERENCE TO SHEAR DEFORMATIONS
DEFLECTION OF BEAMS WlTH SPECIAL REFERENCE TO SHEAR DEFORMATIONS THE INFLUENCE OF THE FORM OF A WOODEN BEAM ON ITS STIFFNESS AND STRENGTHI (REPRINT FROM NATIONAL ADVISORY COMMITTEE FOR AERONAUTICS REPORT
More informationThe Torsion Pendulum (One or two weights)
The Torsion Pendulum (One or two weights) Exercises I through V form the oneweight experiment. Exercises VI and VII, completed after Exercises I V, add one weight more. Preparatory Questions: 1. The
More informationSupport Idealizations
IVL 3121 nalysis of Statically Determinant Structures 1/12 nalysis of Statically Determinate Structures nalysis of Statically Determinate Structures The most common type of structure an engineer will analyze
More informationFLAC3D analysis on soil moving through piles
University of Wollongong Research Online Faculty of Engineering  Papers (Archive) Faculty of Engineering and Information Sciences 211 FLAC3D analysis on soil moving through piles E H. Ghee Griffith University
More informationCEE 271: Applied Mechanics II, Dynamics Lecture 9: Ch.13, Sec.45
1 / 40 CEE 271: Applied Mechanics II, Dynamics Lecture 9: Ch.13, Sec.45 Prof. Albert S. Kim Civil and Environmental Engineering, University of Hawaii at Manoa 2 / 40 EQUATIONS OF MOTION:RECTANGULAR COORDINATES
More informationUNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation.
UNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The magnitude
More informationEquilibrium in Two Dimensions
C h a p t e r 6 Equilibrium in Two Dimensions In this chapter, you will learn the following to World Class standards: 1. The Ladder Against the Wall 2. The Street Light 3. The Floor Beam 61 The Ladder
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationCOUPLED USE OF FEA AND EMA FOR THE INVESTIGATION OF DYNAMIC BEHAVIOUR OF AN INJECTION PUMP
COUPLED USE OF FEA AND EMA FOR THE INVESTIGATION OF DYNAMIC BEHAVIOUR OF AN INJECTION PUMP Yasar Deger Wolfram Lienau Peter Sandford Sulzer Markets & Sulzer Pumps Ltd Sulzer Pumps (UK) Ltd Technology Ltd
More informationFRACTURE MECHANICS FOR MEMBRANES
FRACTURE MECHANICS FOR MEMBRANES Chong Li, Rogelio Espinosa and Per Ståhle Solid Mechanics, Malmö University SE 205 06 Malmö, Sweden chong.li@ts.mah.se Abstract During fracture of membranes loading often
More informationGlossary Innovative Measurement Solutions
Glossary GLOSSARY OF TERMS FOR TRANSDUCERS, LOAD CELLS AND WEIGH MODULES This purpose of this document is to provide a comprehensive, alphabetical list of terms and definitions commonly employed in the
More informationCH. 5 TRUSSES BASIC PRINCIPLES TRUSS ANALYSIS. Typical depthtospan ratios range from 1:10 to 1:20. First: determine loads in various members
CH. 5 TRUSSES BASIC PRINCIPLES Typical depthtospan ratios range from 1:10 to 1:20  Flat trusses require less overall depth than pitched trusses Spans: 40200 Spacing: 10 to 40 on center  Residential
More informationFigure 1: Throwing arm dimensions
I. Overview The objective of this report is to review the design of the trebuchet model from an engineering standpoint. This study analyzes the dimensions and material selection using the COMSOL multiphisics
More informationVIBRATION ANALYSIS OF TIEROD/TIEBOLT ROTORS USING FEM
VIBRATION ANALYSIS OF TIEROD/TIEBOLT ROTORS USING FEM J. E. Jam, F. Meisami Composite Materials and Technology Center Tehran, IRAN jejaam@gmail.com N. G. Nia Iran Polymer & Petrochemical Institute, Tehran,
More informationExam paper: Biomechanics
Exam paper: Biomechanics Tuesday August 10th 2010; 9.0012.00 AM Code: 8W020 Biomedical Engineering Department, Eindhoven University of Technology The exam comprises 10 problems. Every problem has a maximum
More informationTOPIC D: ROTATION EXAMPLES SPRING 2018
TOPIC D: ROTATION EXAMPLES SPRING 018 Q1. A car accelerates uniformly from rest to 80 km hr 1 in 6 s. The wheels have a radius of 30 cm. What is the angular acceleration of the wheels? Q. The University
More informationCode_Aster. Calculation algorithm of the densities of reinforcement
Titre : Algorithme de calcul des densités de ferraillage Date : 05/08/2013 Page : 1/11 Calculation algorithm of the densities of reinforcement Summary: One presents the calculation algorithm of the densities
More informationStress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole
Stress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole Dheeraj Gunwant, J. P. Singh mailto.dheerajgunwant@gmail.com, jitenderpal2007@gmail.com, AIT, Rampur Abstract A static
More informationThe Torsion Pendulum
Page 1 of 9 The Torsion Pendulum Introduction: This experiment helps to relate many of the concepts that we see in everyday life. Damped oscillations and pendulums are an everyday occurrence. You will
More informationAnnouncements. Principle of Work and Energy  Sections Engr222 Spring 2004 Chapter Test Wednesday
Announcements Test Wednesday Closed book 3 page sheet sheet (on web) Calculator Chap 12.610, 13.16 Principle of Work and Energy  Sections 14.13 Today s Objectives: Students will be able to: a) Calculate
More informationUNIT I SIMPLE STRESSES AND STRAINS
Subject with Code : SM1(15A01303) Year & Sem: IIB.Tech & ISem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES
More informationMENG 302L Lab 6: Stress Concentration
Introduction 1 : The purpose of this experiment is to demonstrate the existence of stress and strain concentration in the vicinity of a geometric discontinuity in a cantilever beam, and to obtain an approximate
More informationChapter 8 Rotational Motion
Chapter 8 Rotational Motion Chapter 8 Rotational Motion In this chapter you will: Learn how to describe and measure rotational motion. Learn how torque changes rotational velocity. Explore factors that
More information1.105 Solid Mechanics Laboratory
1.105 Solid Mechanics Laboratory General Information Fall 2003 Prof. Louis Bucciarelli Rm 5213 x34061 llbjr@mit.edu TA: Attasit Korchaiyapruk, Pong Rm 5330B x 35170 attasit@mit.edu Athena Locker: /mit/1.105/
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 3
MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.
More informationDEVELOPMENT OF DROP WEIGHT IMPACT TEST MACHINE
CHAPTER8 DEVELOPMENT OF DROP WEIGHT IMPACT TEST MACHINE 8.1 Introduction The behavior of materials is different when they are subjected to dynamic loading [9]. The testing of materials under dynamic conditions
More informationVerification of Numerical Modeling in Buried Pipelines under Large Fault Movements by SmallScale Experiments
Verification of Numerical Modeling in Buried Pipelines under Large Fault Movements by SmallScale Experiments T.J. Lin, G.Y. Liu, L.L. Chung, and C.H. Chou National Center for Research on Earthquake Engineering,
More informationCOLUMN BASE WEAK AXIS ALIGNED ASYMMETRIC FRICTION CONNECTION CYCLIC PERFORMANCE
8 th International Conference on Behavior of Steel Structures in Seismic Areas Shanghai, China, July 13, 2015 COLUMN BASE WEAK AXIS ALIGNED ASYMMETRIC FRICTION CONNECTION CYCLIC PERFORMANCE J. Borzouie*,
More informationTABLE OF CONTENT Scope 2 Alignment Systems and Procedures 2 Balancing 8 Lubrication System 10 Preservation of Spare Parts 12
Page : 1 of 21 Project Engineering Standard www.klmtechgroup.com KLM Technology #0312 Block Aronia, Jalan Sri Perkasa 2 Taman Tampoi Utama 81200 Johor Bahru Malaysia TABLE OF CONTENT Scope 2 Alignment
More informationRESEARCH PROJECT NO. 26
RESEARCH PROJECT NO. 26 DETERMINATION OF POISSON'S RATIO IN AD1 TESTING BY UNIVERSITY OF MICHIGAN REPORT PREPARED BY BELA V. KOVACS and JOHN R. KEOUGH \ MEMBER / / DUCTILE IRON \ SOCIETY Issued by the
More informationKINGS COLLEGE OF ENGINEERING ENGINEERING MECHANICS QUESTION BANK UNIT I  PARTA
KINGS COLLEGE OF ENGINEERING ENGINEERING MECHANICS QUESTION BANK Sub. Code: CE1151 Sub. Name: Engg. Mechanics UNIT I  PARTA Sem / Year II / I 1.Distinguish the following system of forces with a suitable
More informationLevers. 558 A Textbook of Machine Design
558 A Textbook of Machine Design C H A P T E R 15 Levers 1. Introduction.. Application of Levers in Engineering Practice.. Design of a Lever. 4. Hand Lever. 5. Foot Lever. 6. Cranked Lever. 7. Lever for
More information2008 FXA THREE FORCES IN EQUILIBRIUM 1. Candidates should be able to : TRIANGLE OF FORCES RULE
THREE ORCES IN EQUILIBRIUM 1 Candidates should be able to : TRIANGLE O ORCES RULE Draw and use a triangle of forces to represent the equilibrium of three forces acting at a point in an object. State that
More informationVALLIAMMAI ENGINEERING COLLEGE SRM NAGAR, KATTANKULATHUR DEPARTMENT OF MECHANICAL ENGINEERING
VALLIAMMAI ENGINEERING COLLEGE SRM NAGAR, KATTANKULATHUR 603203 DEPARTMENT OF MECHANICAL ENGINEERING BRANCH: MECHANICAL YEAR / SEMESTER: I / II UNIT 1 PART A 1. State Newton's three laws of motion? 2.
More informationPullout Tests of Geogrids Embedded in Noncohesive Soil
Archives of HydroEngineering and Environmental Mechanics Vol. 51 (2004), No. 2, pp. 135 147 Pullout Tests of Geogrids Embedded in Noncohesive Soil Angelika Duszyńska, Adam F. Bolt Gdansk University of
More informationElasticity: Term Paper. Danielle Harper. University of Central Florida
Elasticity: Term Paper Danielle Harper University of Central Florida I. Abstract This research was conducted in order to experimentally test certain components of the theory of elasticity. The theory was
More informationASSOCIATE DEGREE IN ENGINEERING EXAMINATIONS. SEMESTER 2 May 2013
ASSOCIATE DEGREE IN ENGINEERING EXAMINATIONS SEMESTER 2 May 2013 COURSE NAME: CODE: Mechanical Engineering Science [8 CHARACTER COURSE CODE] GROUP: ADENG 1 DATE: TIME: DURATION: "[EXAM DATE]" "[TIME OF
More informationQuestion Figure shows the strainstress curve for a given material. What are (a) Young s modulus and (b) approximate yield strength for this material?
Question. A steel wire of length 4.7 m and crosssectional area 3.0 x 105 m 2 stretches by the same amount as a copper wire of length 3.5 m and crosssectional area of 4.0 x 105 m 2 under a given load.
More informationMECTROL CORPORATION 9 NORTHWESTERN DRIVE, SALEM, NH PHONE FAX TIMING BELT THEORY
MECTRO CORPORATION 9 NORTHWESTERN DRIVE, SAEM, NH 03079 PHONE 60389055 FAX 60389066 TIMING BET THEORY Copyright 997, 999, 00 Mectrol Corporation. All rights reserved. April 00 Timing Belt Theory Introduction
More informationChapter I 1 FRACTURING AROUND A ROCK BOLT ANCHOR. by Richard S. Culver and Tron Jorstad
Chapter I 1 FRACTURING AROUND A ROCK BOLT ANCHOR by Richard S. Culver and Tron Jorstad In spite of the widespread interest in rock bolt research, relatively little is known about the critical region surrounding
More information3D Force Couple System and Resultant. Q.No.1: Replace the force system by an equivalent force and couple moment at point A.
3D Force Couple System and Resultant Q.No.1: Replace the force system by an equivalent force and couple moment at point A. Q.No.2: Handle forces F1 and F2 are applied to the electric drill. Replace this
More informationMECHANICS OF SOLIDS Credit Hours: 6
MECHANICS OF SOLIDS Credit Hours: 6 Teaching Scheme Theory Tutorials Practical Total Credit Hours/week 4 0 6 6 Marks 00 0 50 50 6 A. Objective of the Course: Objectives of introducing this subject at second
More information2014 MECHANICS OF MATERIALS
R10 SET  1 II. Tech I Semester Regular Examinations, March 2014 MEHNIS OF MTERILS (ivil Engineering) Time: 3 hours Max. Marks: 75 nswer any FIVE Questions ll Questions carry Equal Marks ~~~~~~~~~~~~~~~~~~~~~~~~~
More informationMET 301 EXPERIMENT # 2 APPLICATION OF BONDED STRAIN GAGES
MET 301 EPERIMENT # 2 APPLICATION OF BONDED STRAIN GAGES 1. Objective To understand the working principle of bonded strain gauge and to study the stress and strain in a hollow cylindrical shaft under bending,
More informationDeflections and Strains in Cracked Shafts Due to Rotating Loads: A Numerical and Experimental Analysis
International Journal of Rotating Machinery, 9: 303 311, 2003 Copyright c Taylor & Francis Inc. ISSN: 1023621X DOI: 10.1080/10236210390147416 Deflections and Strains in Cracked Shafts Due to Rotating
More informationFinite Element Modelling with Plastic Hinges
01/02/2016 Marco Donà Finite Element Modelling with Plastic Hinges 1 Plastic hinge approach A plastic hinge represents a concentrated postyield behaviour in one or more degrees of freedom. Hinges only
More informationQ16.: A 5.0 kg block is lowered with a downward acceleration of 2.8 m/s 2 by means of a rope. The force of the block on the rope is:(35 N, down)
Old Exam Question Ch. 5 T072 Q13.Two blocks of mass m 1 = 24.0 kg and m 2, respectively, are connected by a light string that passes over a massless pulley as shown in Fig. 2. If the tension in the string
More information7.4 The Elementary Beam Theory
7.4 The Elementary Beam Theory In this section, problems involving long and slender beams are addressed. s with pressure vessels, the geometry of the beam, and the specific type of loading which will be
More informationThe Local Web Buckling Strength of Coped Steel IBeam. ABSTRACT : When a beam flange is coped to allow clearance at the
The Local Web Buckling Strength of Coped Steel IBeam Michael C. H. Yam 1 Member, ASCE Angus C. C. Lam Associate Member, ASCE, V. P. IU and J. J. R. Cheng 3 Members, ASCE ABSTRACT : When a beam flange
More informationMeasurement of Bone Strength and Stiffness using 3Point Bending
BME 315 Biomechanics, U. Wisconsin Adapted by R. Lakes from D. Thelen and C. Decker, 09, adapted from Lakes 06 Experimental Details I. Laboratory equipment The load frame that we will use to perform our
More informationUse the following to answer question 1:
Use the following to answer question 1: On an amusement park ride, passengers are seated in a horizontal circle of radius 7.5 m. The seats begin from rest and are uniformly accelerated for 21 seconds to
More informationChapter 1 Introduction Concept of Stress
hapter 1 Introduction oncept of Stress INTRODUTION Review of Statics xial Stress earing Stress Torsional Stress 14 6 ending Stress W W L Introduction 11 Shear Stress W W Stress and Strain L y y τ xy
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationQuestion 9.1: A steel wire of length 4.7 m and crosssectional area 3.0 10 5 m 2 stretches by the same amount as a copper wire of length 3.5 m and crosssectional area of 4.0 10 5 m 2 under a given load.
More informationRutgers University Department of Physics & Astronomy. 01:750:271 Honors Physics I Fall Lecture 19. Home Page. Title Page. Page 1 of 36.
Rutgers University Department of Physics & Astronomy 01:750:271 Honors Physics I Fall 2015 Lecture 19 Page 1 of 36 12. Equilibrium and Elasticity How do objects behave under applied external forces? Under
More information2012 Road School Light Weight Deflectometer (LWD)
2012 Road School Light Weight Deflectometer (LWD) Nayyar Siddiki, M.S., P.E. Office of Geotechnical Services Outline Testing for Compaction NO 53 and chemically modified soils (Special Prov.) Changing
More information